Introduction to Rheology Basics

 Jeffery Elijah Norris
 9 months ago
 Views:
Transcription
1 Introduction to Rheology Basics RheoTec Messtechnik GmbH Phone: ++49 (035205) Schutterwaelder Strasse 23 Fax: ++49 (035205) D OttendorfOkrilla Germany Internet:
2 1 Content 1 Fundamental rheological terms Introduction Definitions Shear stress Shear rate Dynamic viscosity Kinematic viscosity Factors which affect the viscosity Loaddependent flow behaviour Newtonian flow behaviour Pseudoplasticity Dilatancy Plasticity and yield point Timedependent flow behaviour Thixotropy Rheopexy Temperaturedependent flow behaviour Flow behaviour of viscoelastic materials Viscoelastic liquids Viscoelastic solids Flow behaviour of elastic materials Strain Shear modulus Rheometry Tests at controlled shear rate (CSR mode) Viscositytime test Viscositytemperature test Flow and viscosity curves Tests at controlled shear stress (CSS mode) Viscositytime test Viscositytemperature test Flow and viscosity curves Creep and recovery test Measuring geometries in a rotation viscometer Coaxial cylinder measuring systems Dualslit measuring systems according to DIN Coneplate measuring systems according to ISO Plateplate measuring systems...47
3 2 1 Fundamental rheological terms 1.1 Introduction Material scientists have investigated the flow and strain properties of materials since the 17 th century. The term rheology was first used in physics and chemistry by E.C. BINGHAM and M. REINER on 29 April 1929 when the American Society of Rheology was founded in Columbus, Ohio. Rheological parameters are mechanical properties. They include physical properties of liquids and solids which describe strain and flow behaviour (temporal variation of strain). Strain is observed in all materials and substances when exerting external forces. Rheometry describes measuring methods and devices used to determine rheological properties. If an external force is exerted on a body, its particles will be displaced relative to each other. This displacement of particles is known as strain. Type and extent of strain are characteristic properties of a body. Ideally elastic bodies undergo elastic strain if external anisotropic forces are exerted on them. The energy needed for this strain is stored and effects spontaneous full recovery of the original form if the external force ceases to act. Ideally viscous bodies undergo an irreversible strain if external anisotropic forces (e.g. gravitational force) are exerted on them. The input energy is transformed. This increasing viscous strain is known as flowing. There are only few fluids with practical importance which show (almost) ideally viscous behaviour. Most materials are neither ideally viscous nor ideally plastic. They rather exhibit different behaviour and are thus called viscoelastic materials.
4 3 The most simple model to illustrate rheological properties is the parallel plate model. The top plate, which has a surface area A [m²], is moved by a force F [N = kgm/s²] at a speed v [m/s]. The bottom plate remains at rest. The distance between the plates, to which the material adheres, is described by h [m]. Now, thinnest elements of the liquid will be displaced between the plates. This laminar flow is of fundamental importance for rheological investigations. Turbulent flows increase the flow resistance, thus showing false rheological properties. A moved plate F v h fix plate Fig. 11: Parallel plate model Shear rate = v / h in s 1 Shear stress τ = F / A in Pa Viscosity η = τ / in Pas Strain γ = dx / h dimensionless In addition to the expression, the symbol D is also used for the shear rate. Shear tests are usually conducted using rotation viscometers. In contrast to the parallel plate model, the moved surface performs a rotary movement.
5 4 1.2 Definitions Shear stress Force F acting on area A to effect a movement in the liquid element between the two plates. The velocity of the movement at a given force is controlled by the internal forces of the material. Shear stress τ = Force F Area A N = ( Newton) m 2 = Pa 100 Pa = 1 mbar = 1 hpa old unit: dyn / cm 2 = 0.1 Pa Shear rate By applying shear stress a laminar shear flow is generated between the two plates. The uppermost layer moves at the maximum velocity v max, while the lowermost layer remains at rest. The shear rate is defined as: Shear rate = dv dh where dv Velocity differential between adjacent velocity layers dh Thickness differential of the flow layers In a laminar flow the velocity differential between adjacent layers of like thickness is constant (dv = const., dh = const.) The differential can thus be approximated as follows: Shear rate = Velocity v Distance h = m/ s m = s 1 In addition to, the symbol D is also used for the shear rate in the literature.
6 5 Process ranges in s 1 Example of use Sedimentation of fine particles in suspensions Paints, lacquers, pharmaceutical solutions Flowing due to surface characteristics Paints, printing inks Dripping under the effect of the gravitational force Paints, coatings Extruding Polymers Chewing/ swallowing Food Spreading butter on a slice of bread Food Mixing, agitating Substances in process engineering Brushing Paints, lacquers, pastes Spraying, spreading Paints, lacquers, coatings Rubbing in Creams, lotions Highspeed coating Paper coatings Lubrication of machine parts Mineral oils, greases Table 11: Typical shear rate ranges
7 Dynamic viscosity Viscosity describes the toughness of a material. Shear stress τ Dynamic viscosity η = Shear rate = Pa s 1 = Pas The unit Pas (or mpas) is used for the viscosity. 1 Pas = 1000 mpas old unit: 1 P (Poise) = 100 cp (Centipoise) = 100 mpas (Millipascalsecond) Substance Dyn. viscosity η in mpas Acetone 0.32 Water 1.0 Ethanol 1.2 Mercury 1.5 Grape juice Cream approx % sugar solution 57 Olive oil: approx. 100 Honey approx. 10,000 Plastic melts Tar approx Bitumen approx Earth mantle approx Table 12: Typical viscosities at 20 C in mpas
8 Kinematic viscosity If ideally viscous materials are tested using a capillary viscometer, such as an UBBELOHDE viscometer, the kinematic viscosity ν is determined, not the dynamic viscosity η. The kinematic viscosity is related to the dynamic viscosity through the density of the material. Dynamic viscosity η mm Kinematic viscosity ν = = Density ρ s 2 Old unit: cst (Centistokes) = mm² / s There used to be several devicespecific measuring methods to determine the kinematic viscosity, e.g. FORD cups, and, accordingly, a large number of units, such as FORD cup seconds, ENGLER degrees, REDWOOD or SAYBOLD units. These viscositydependent values cannot be converted into absolute viscosities η or ν for nonnewtonian fluids.
9 8 1.3 Factors which affect the viscosity The flow and strain behaviour of a material may be affected by a number of external factors. The five most important parameters are: Substance The viscosity of a material depends on its physical and chemical properties. Temperature Temperature has a major effect on the viscosity. For example, several mineral oils lose about 10 % of their viscosity if the temperature is only increased by 1 K. Shear rate The viscosity of most materials depends on the shear rate, i.e. the load. Time The viscosity depends on the strain history of a material, in particular on previous loads. Pressure If great pressure is exerted on a material, its viscosity may increase as particles are organised in a more tight structure (resulting in more interaction possibilities). Other influencing factors are the ph value, magnetic and electric field strength.
10 9 2 Loaddependent flow behaviour Flow and viscosity curves The flow behaviour of a material is characterised by the relation between shear stress τ and shear rate. A τ diagram is often used for graphic representation. Usually, the shear stress is shown on the ordinate and the abscissa the shear rate, irrespective of whether or τ were given for the measurement. These diagrams are referred to as flow functions or flow curves. τ [Pa] [s 1 ] Fig. 21: Flow curve Plotting the viscosity over the shear rate or shear stress τ produces the viscosity function or viscosity curve. η [mpas] [s 1 ] Fig. 22: Viscosity curve The measuring result obtained with a viscometer or rheometer is always a flow curve. However, the viscosity function can be calculated based on the measured values.
11 Newtonian flow behaviour If a NEWTONian material is subjected to a shear stress τ, a shear gradient of viscous flow is generated which is proportional to the applied shear stress. The flow function of a NEWTONian material is a straight line which runs through the origin of the coordinate system at an angle α. This relation between shear stress and shear gradient is described by NEWTON s law of viscosity. τ η = = const. η is the material constant of the dynamic shear viscosity. If the viscosity is plotted over the shear rate (or shear stress) in a viscosity diagram, a straight line which starts at = 0 s 1 (or τ = 0 Pa) and runs parallel to the abscissa is obtained for an ideally viscous material. τ η Fig. 23: Flow curves of NEWTONian materials Fig. 24: Viscosity curves of NEWTONian materials The viscosity of a NEWTONian material or ideally viscous material is independent of the shear rate. Examples of NEWTONian materials: water, mineral oil, sugar solution, bitumen
12 11 According to NEWTON, a viscous body may be represented by the mechanical model of a damper. Force F Fig. 25: Mechanical model of a NEWTONian body It can be shown with the help of this model that the material is continuously deformed in the damper as long as a force acts on the piston. If the force ceases to act, the original shape is not restored. A viscous strain is characterised in that the energy input to create a flow is fully transformed into heat in an irreversible process. Materials which show only little interaction between (usually short) molecules exhibit NEWTONian flow behaviour.
13 Pseudoplasticity Many materials exhibit a strong decrease in viscosity if the shear rate grows. This effect is of great technical importance. Compared with an ideally viscous material, a pseudoplastic or structurally viscous material can be pumped through pipelines with a lower energy input at the same flow velocity. τ / = η const. The proportionality factor τ / in the NEWTONian constitutive equation is thus referred to as η a. η a is the apparent viscosity and denotes the viscosity at a certain shear rate. Mathematical expression for pseudoplastic materials according to OSTWALD DE WAELE: τ = K n where n < 1 for pseudoplastic materials Transformed into a viscosity function: η = τ = K n 1 τ η Fig. 26: Flow curve of a pseudoplastic material Fig. 27: Viscosity curve of a pseudoplastic material Examples: suspensions, dispersions, paints, lacquers, creams, lotions, gels Materials are referred to as pseudoplastic if a force acting on the body causes the particle size to change, the particles to be oriented in the direction of flow, or an agglomerate to be dissolved.
14 Dilatancy The viscosity of dilatant materials also depends on the shear rate. It increases as the shear rate grows. Dilatant behaviour can cause trouble in technological processes. Mathematical expression according to OSTWALD DE WAELE: τ = K n where n > 1 for dilatant materials Transformed into a viscosity function: η = τ = K n+ 1 τ η Fig. 28 Flow curve of a dilatant material Fig. 28 Viscosity curve of a dilatant material Dilatant behaviour is found rather seldom. Examples: concentrated corn starch dispersions, wet sand, several ceramic suspensions, several surfactant solutions Note: If in case of high shear rates the flow in the measuring gap is no longer laminar, but becomes turbulent, this may falsely suggest dilatant behaviour.
15 Plasticity and yield point Plasticity describes structurally viscous liquids which have an additional yield point τ o. A practical example of such a material is toothpaste. At rest, toothpaste establishes an network of intermolecular bonding forces. These forces prevent individual volume elements to be displaced when the material is at rest. If an external force which is smaller than the internal forces (bonding forces) acts on the material, the resulting strain is reversible, as with solids. However, if the external forces exceed the internal bonding forces of the network, the material will start flowing, the solid turns into a liquid. Definition of the yield point τ o Maximum shear stress τ at the shear rate = 0 s 1 Thus, if F external < F internal, the material does not flow if F external > F internal, the material starts to flow Examples: Toothpaste, PVC paste, emulsion paint, lipstick, fats, printing ink, butter Flow curves and mathematical expression of materials with a yield point Flow curves of plastic liquids do not start in the origin of the coordinate system, but run on the ordinate axis until the yield point τ o is reached, then they converge from the ordinate. The flow curves can be expressed mathematically using a number of equations, depending on the actual material. For example, the flow curve of chocolate is typically based on the CASSON model. Mathematical expression according to BINGHAM: τ = f B + η B (where f B = yield point according to BINGHAM) Mathematical expression according to CASSON: τ = f C + η C (where f C = yield point according to CASSON) Mathematical expression according to HERSCHEL and BULKLEY: τ = f H + m p (where f H = yield point according to HERSCHEL and BULKLEY) where p < 1 for pseudoplastic and p > 1 for dilatant materials
16 15 τ τ τ o τ o Fig. 210: Flow curve according to BINGHAM Fig. 211: Flow curve according to HERSCHEL and BULKLEY Physical causes for the occurrence of yield points in dispersions are intermolecular particleparticle and particledispersing agent interactions.  VAN DER WAALS forces  Dipoledipole interactions  Hydrogen bonds  Electrostatic interactions The ST. VENANT model (with static friction) is a mechanical model used to describe plastic behaviour. Fig. 212: ST. VENANT model for plastic materials
17 16 3 Timedependent flow behaviour 3.1 Thixotropy Thixotropy is a property exhibited by nonnewtonian liquids, they return to their original viscosity only with a delay after the shear force ceased to act. In addition, these materials often also have a yield point. Tomato ketchup is an example of such a material. When stirred or shaken, ketchup becomes thinner and only returns to its original viscosity after allowing to rest for a while. Per definition, a thixotropic material does not only thin depending on the shear rate, but it additionally returns to its original viscosity after a materialspecific period of rest. Theses gelsol and solgel changes in thixotropic materials are reproducible. Yoghurt serves as a counterexample: it becomes thinner when stirred, but does not return to its original thickness. Yoghurt thus does not exhibit thixotropic flow behaviour. η Shear at = const. Sample at rest ( = 0.1 s 1 ) Fig. 31: Viscositytime curve of a thixotropic material t Two transitional areas can be easily identified in the viscositytime curve shown above. A gel is quickly transformed into a sol at a constant shear force. During the period of rest the materialspecific network structures are reestablished, i.e. the sol turns back into a gel.
18 17 τ UP η UP DOWN DOWN Fig. 32: Flow and viscosity curve of a pseudoplastic and a thixotropic material The flow curve shows that the measured rising and declining curves are not congruent. The area between the two curves (hysteresis area) defines the extent of the timedependent flow behaviour. The larger the area the more thixotropic is the material. Examples: paints, foodstuff, cosmetics, pastes
19 Rheopexy Rheopectic materials exhibit greater viscosity while they are subject to shear stress. Structures are established in the material during the application of mechanical shear forces. The original viscosity is only restored with a delay after the shear forces ceased to act on the material, by disintegrating this structure. η Shear at = const. Sample at rest ( = 0.1 s 1 ) Fig. 33: Viscositytime curve of a rheopectic material t This process of viscosity increase and decrease can be repeated as often as you wish. In contrast to thixotropy, true rheopexy is very rare. τ η UP UP DOWN DOWN Fig. 34: Flow and viscosity curve of a pseudoplastic and a rheopectic material Examples: several latex dispersions, several casting slips, several surfactant solutions
20 19 4 Temperaturedependent flow behaviour As mentioned above, the viscosity of a material is a function of temperature. Exact temperature control and accurate indication of the measuring temperature is thus of major importance in viscosity measurements. The viscositytemperature curve of a material is found at a constant shear rate. In most materials, the viscosity decreases as the temperature is raised. In ideally viscous materials, this phenomenon can be described with the help of the ARRHENIUS equation: η = A e B T where T... temperature in Kelvin A, B.. material constants η T Fig. 41: Viscositytemperature curve Viscositytemperature curves are also often established in order to trace certain reactions. For example, the curing temperature can be determined for powder lacquers (see Fig. 42, curve a), or the chocolate melting process can be followed (see Fig. 42, curve b). η a b T Fig. 42: Viscositytemperature curves of certain reactions
21 20 5 Flow behaviour of viscoelastic materials Viscoelastic materials exhibit both viscous and elastic properties. Because of physical differences, a distinction is made between viscoelastic liquids and viscoelastic solids. The elastic portion of viscoelastic liquids is described by HOOKE S law, which is also known as the spring model, the viscous portion by NEWTON S damper model. 5.1 Viscoelastic liquids Viscoelastic materials and purely viscous materials can only be distinguished if they are stirred, for example. Rheological phenomena cannot be observed while they are at rest. In a viscous liquid, a rotating agitator causes centrifugal forces, which drive volume elements of the liquid towards the wall of the cup. This means that a dip is formed around the agitator shaft. In contrast, in elastic liquids the rotating agitator causes normal forces which are so great that they do not only compensate the centrifugal forces but exceed them. Consequently, volume elements of the liquid are thus dawn up the agitator shaft. This phenomenon of masses creeping up a rotating shaft due to the acting normal forces is called the WEISSENBERG effect. Fig. 51: Flow behaviour of a viscous and a viscoelastic liquid A force acting on a viscoelastic material (see Fig. 52) causes the spring to be deformed immediately, but the damper reacts with a delay. If the force ceases to act, the spring will return immediately while the damper remains displaced, so that the material partly remains strained. That means that there is no full restoration of shape. The amount of the spring return corresponds with the elastic portion, the amount of the remaining strain (damper) corresponds with the viscous portion. A viscoelastic liquid can thus be described using a model where damper and spring are arranged in series. Honouring JAMES C. MAXWELL ( ), this series connection is also called the MAXWELL model.
22 21 Fig. 52: Maxwell model Examples of viscoelastic liquids are gels and silicone rubber compounds 5.2 Viscoelastic solids If a force is exerted on a viscoelastic solid a delayed strain will take place, because the displacement of the spring is impeded by the damper. If the force ceases to be exerted, the body will fully return to its original shape (but again delayed by the damper). That means that there is a full restoration of shape. It can thus be said that a viscoelastic solid is characterised in that it has the ability of reversible strain. The model to describe such materials is again a combination of spring and damper models. In contrast to viscoelastic liquids, however, the two elements are connected in parallel, as in the KELVINVOIGT model. Fig. 53: KELVINVOIGT model An example of a viscoelastic solid is hard rubber.
23 22 6 Flow behaviour of elastic materials 6.1 Strain A cube with an edge length h shall be investigated here as the volume element in order to illustrate the strain γ. The bottom face of the volume element is fixed. A force F acts on its top face, which is thereby displaced by the amount s. F s h h α Fig. 61: Unloaded volume element Loaded volume element Mathematical expression: s tan α = = γ h Strain is a dimensionless parameter. A deformation angle α of 45 corresponds with a strain γ of 1 or 100%. The symbol for the shear rate ( ) can be derived from that for the strain (γ). The shear rate describes the strain change dγ during a period of time dt. Consequently, is the derivative of strain γ with respect to time t. In other words, the shear rate can be considered to be the strain rate. 6.2 Shear modulus In purely elastic bodies, the ratio of shear stress τ and resulting strain γ is constant. This materialspecific parameter described the stiffness of the material and is known as the shear modulus G. Shear stress τ Pa Shear modulus G = = = Pa Strain γ 1 The shear modulus can be in the MPa (10 6 Pa) range in very stiff bodies.
24 23 7 Rheometry Viscometers or rheometers used to determine the rheological properties are called absolute viscometers if the measured values are based on the basic physical units of force [N], length [m] and time [s]. dynamic viscosity η = [N/m 2 ] [s] = force / length 2 time = [Pa] [s] Viscometers are measuring devices which are used to determine the viscosity depending on the rotational speed (= shear rate), time and temperature. Rheometers are devices which are additionally able to determine the viscous and viscoelastic product properties depending on the force (shear stress) exerted in both rotation/ creep test and oscillation test. Absolute viscometers have the advantage that the results of the measurements are independent of the device manufacturer or measuring equipment used. The material under investigation is filled into the twopart measuring system, where a shear force is applied. The measurements must be conducted under certain boundary conditions in order to obtain correct results. The applied shear force must only produce a stratified laminar flow. Vortices and turbulences in the measuring system consume much energy so that viscosity values up to 40 % above the true viscosity are obtained. The material under investigation should be homogeneous. It is not recommended to mix substances during the measurement. Due to the different specific weights of the components a phase separation of the mix may occur during the measurement. The changed composition of the mix in the measuring gap may lead to erroneous viscosity values. The material must adhere to the walls. The force exerted on the top plate must be fully transmitted on to the sample. This condition is not fulfilled if the boundary layers of the material under investigation do not properly adhere to the parts of the measuring system. Problems in this respect may be encountered with materials such as fats. The elasticity of the sample must not be too high. The shear forces acting on the sample may otherwise result in extreme normal forces such that the material creeps out of the measuring gap. When handling elastic materials, the shear rate must be chosen such that normal stress does not affect the measuring result. The shear stress applied according to the laws of viscosity is proportional to the shear rate and shall only be as great as is necessary to maintain stationary flow conditions, i.e. a flow at constant velocity. The force that is necessary to accelerate or decelerate the flow is not considered in this equation. The NEWTONian relation η = τ / shows that the viscosity η can be determined using either of two different measuring methods.
25 Tests at controlled shear rate (CSR mode) (CSR controlled shear rate) With this measuring method, the rotational speed n is preset at the rheometer, and the shear rate is calculated based on the gap h and the rotational speed n (or circumferential speed v of the shearing area). The flow resistance moment M (or the shear force F) of the braking, tough material under investigation is measured. This torque M is converted into the rheological parameter of shear stress using the shear area A of the measuring system. physical setting rheological setting rot. speed n [min 1 ] shear rate [s 1 ] measurement physical result torque M [mnm] rheological result shear stress τ [Pa] η = τ The dynamic viscosity η is calculated from the shear stress τ and shear rate (or D).
26 Viscositytime test A constant shear rate is applied for a certain period of time. The shear stress τ is measured as a function of time. The viscosity determined according to the viscosity equation is obtained in relation to time. This test is used in practice in stability investigations, to study hardening reactions and with thixotropic materials. [s 1 ] t [s] Fig. 71: Conditions: shear rate = const., temperature = const. τ [Pa] 3 η [Pas] t [s] t [s] 1 Material with a viscosity which does not change over time (e.g. calibration oil) 2 Material with a viscosity which decreases over time (e.g. ketchup) 3 Material with a viscosity which increases over time (e.g. hardening lacquer) Fig. 72: Results of the viscositytime tests
27 Viscositytemperature test At a constant shear rate, a temperature ramp is preset and the viscosity is measured in relation to temperature. In practice, this test is conducted when it comes to investigating temperaturedependent hardening or melting reactions. T [ C] Fig. 73: Conditions: shear rate = const., variable temperature t [s] τ [Pa] 2 η [Pas] T [ C] T [ C] 1 Material with a viscosity which decreases as the temperature rises (e.g. chocolate) 2 Material with a viscosity which increases as the temperature rises (e.g. hardening lacquer) Fig. 74: Results of the viscositytemperature tests
28 Flow and viscosity curves At a constant temperature, a shear rate  time profile is preset. The shear stress is measured for each shear rate value and the corresponding viscosity is calculated from those measuring results. [s1 ] T=const. t [s] Fig. 75: Conditions: variable shear rate, temperature = const. A constant viscosity value is found in materials with ideally viscous behaviour (NEWTONian materials), such as water. In materials with pseudoplastic behaviour the viscosity decreases as the shear rate rises ( shear thinning ). In contrast, in materials with dilatant behaviour the viscosity increases as the shear rate rises ( shear thickening ). τ [Pa] η [Pas] [s 1 ] [s 1 ] 1 NEWTONian material 2 Pseudoplastic material 3 Plastic material 4 Dilatant material Fig. 76: Flow and viscosity curves of materials with different rheological behaviour
29 28 Flow and viscosity curves are often plotted such that the viscosity values are shown at both rising and falling shear rate. Between the two sections of the curve (up ramp, down ramp) there is often a section where the shear rate is kept constant. [s 1 ] Fig. 77: Conditions t [s] In addition to loaddependent flow behaviour (pseudoplasticity, dilatancy), the results of the measurements then also allow information about timedependent flow behaviour to be derived. In practice, the area between the up and down curves is often used as a measure for timedependent flow properties, i.e. for the thixotropy of the material. Materials which require a long time after maximum shear to reestablish their structure show in the diagram a large area between the two curves (hysteresis area). τ UP η UP DOWN DOWN Fig. 78: Flow and viscosity curve of a pseudoplastic and a thixotropic material
30 29 In order to be able to compare measured curves with respect to the hysteresis areas, an identical measuring profile must be selected for the individual measurements, i.e. the duration of the individual test phases, the total test duration, the shear rate profile and the temperature must be identical. In addition to pseudoplastic behaviour, thixotropic behaviour can also facilitate certain materials to be processed. Thanks to the reduced viscosity over time, there is less power required for pumping, mixing, spraying or brushing. An advantage of thixotropic coatings is that they spread more smoothly after application and bubbles which are possibly created during the application process can escape more easily. Pseudoplasticity and thixotropy are two rheological properties which exist fully independent of each other. They should not be mistaken.
31 Tests at controlled shear stress (CSS mode) (CSS controlled shear stress) In controlled shear stress tests, the torque M is preset at the rheometer, and the shear stress τ is calculated from the torque M and the shear area A of the measuring system. The rotational speed n achieved by the plunger due to the applied torque is measured. This rotational speed n is converted into the rheological parameter of shear rate using the appropriate measuring system factor. physical setting torque M [mnm] rheological setting shear stress τ [Pa] measurement physical result rot. speed n [min 1 ] rheological result shear rate [s 1 ] η = τ The dynamic viscosity η is calculated from the shear stress τ and shear rate.
32 Viscositytime test A constant shear stress τ is applied to the material under investigation for a certain period of time. The achieved shear rate is measured as a function of time. The viscosity determined according to the viscosity equation is obtained in relation to time. This test is applied in practice when studying hardening reactions. It boasts an advantage over the controlled shear rate test: during hardening the viscosity of the material increases and at a constant shear stress the shear rate falls. This gradually reduces the foreign movement which interferes with the hardening process. τ [Pa] t [s] Fig. 79: Conditions: shear stress = const., temperature = const. [s 1 ] 2 η [Pas] t [s] t [s] 1 Material with a viscosity which does not change over time (e.g. calibration oil) 2 Material with a viscosity which decreases over time (e.g. ketchup) 3 Material with a viscosity which increases over time (e.g. hardening lacquer) Fig. 710: Results of the viscositytime tests
33 Viscositytemperature test At a constant shear stress, a temperature ramp is preset and the viscosity is measured in relation to temperature. In practice, this test is conducted when it comes to investigating temperaturedependent hardening or melting reactions. T [ C] τ = const. t [s] Fig. 711: Conditions: shear stress = const., variable temperature [s 1 ] 1 η [Pas] T [ C] T [ C] 1 Material with a viscosity which decreases as the temperature rises (e.g. chocolate) 2 Material with a viscosity which increases as the temperature rises (e.g. jellying starch) Fig. 712: Results of the viscositytemperature tests
34 Flow and viscosity curves At a constant temperature, a shear stress  time profile is preset. The shear rate is measured for each shear stress value and the corresponding viscosity is calculated from those measuring results. τ [Pa] T=const. t [s] Fig. 713: Conditions: variable shear stress, temperature = const. A constant viscosity value is found in materials with ideally viscous behaviour (NEWTONian materials), such as water. In materials with pseudoplastic behaviour the viscosity decreases as the shear stress rises. In contrast, in materials with dilatant behaviour the viscosity increases as the shear stress rises. τ [Pa] η [Pas] [s 1 ] [s 1 ] 1 NEWTONian material 2 Pseudoplastic material 3 Plastic material 4 Dilatant material Fig. 714: Flow and viscosity curves of materials with different rheological behaviour:
35 34 In mathematics, the given parameter is usually plotted on the abscissa, and the resulting parameter on the ordinate. In contrast, in rheology is plotted on the abscissa and τ on the ordinate, irrespective of whether shear rate or shear stress are given for the measurement. The shear stress test is the only measuring method where the yield point can be determined metrologically. Only if the applied shear stress exceeds the network bonding forces in the material under investigation the material will start to flow, i.e. a measurable shear rate is obtained. In the flow curve shown in Fig. 76, material 3 exhibits a yield point. The flow curve does not pass the origin of the coordinate system, but shows a certain translation on the Y axis. In plastic materials an additional shear stress is required in order to obtain a shear rate in the material. Also in controlled shear stress tests, flow and viscosity curves are often plotted such that the viscosity values are shown at both rising and falling shear stress. Between the two sections of the curve (up ramp, down ramp) there is often a section where the shear stress is kept constant. τ [Pa] T=const. t [s] Fig. 715: Conditions In addition to the yield point value (if any), the results of the measurements then also allow information about loaddependent flow behaviour (pseudoplasticity, dilatancy), and timedependent flow behaviour (thixotropy, rheopexy) to be derived.
36 35 τ UP η UP DOWN DOWN Fig. 716: Flow and viscosity curve of a pseudoplastic and a thixotropic material In order to be able to compare measured curves with respect to the hysteresis areas, which provides information about the thixotropic or rheopectic behaviour of a material, an identical shear rate range should be selected for the individual measurements, and the duration of the individual test phases, the total test duration and the temperature must be identical. As various shear rates can result from a shear stress setting, a shear stress controlled measurement is less suitable for comparing hysteresis areas than a shear rate controlled test. The amount of thixotropy and rheopexy is determined from the flow curves by finding the difference between the areas under the up and down sections of the curve. Thixotropic materials have positive, rheopectic materials negative values.
37 Creep and recovery test The creep test forms a simple and quick method used to find the viscoelastic properties of the material under investigation (with exact distinction between the viscous and elastic portions). The mobile part of the measuring arrangement is loaded with a constant shear stress (τ x ) for a certain period of time (t 0 bis t 2 ). The sample reacts on this force with a deformation, i.e. the material starts to creep. In the second part of the test (t 2 bis t 4 ), the material is relieved from the shear stress so that it can recover. τ [Pa] τ x t 0 t 2 t 4 t [s] Fig. 717: Creep and recovery test Ideally elastic materials A piece of vulcanised rubber will be now be looked at as an example for an ideally elastic material. The constant shear stress applied leads to a certain twist in the sample, i.e. it shows the strain γ. The angle of such strain is characterised by the spring modulus of elasticity of the purely elastic solid. Shear stress and resulting strain γ show a linear relation. If the force is doubled, the strain will also double. HOOKE s spring model serves as a model for ideally elastic materials. The strain is maintained as long as the deforming force keeps acting. 100 % of the strain energy is stored in the spring. The sample will be 100 % relieved if the force ceases to be exerted.
38 37 γ t 0 t 2 t 4 t [s] Fig. 718: Creep and recovery curve of an ideally elastic material (according to HOOKE) Ideally viscous material Serving as an example for a material with ideally viscous behaviour, water shows a completely different behaviour. The constant shear stress applied leads to a strain γ which increases linearly over time, i.e. it shows flowing. The input energy is used up for the flowing process. If the sample is relieved, the strain γ obtained by this moment of time will be maintained. NEWTON s damper model is used to describe an ideally viscous material. γ t 0 t 2 t 4 t [s] Fig. 719: Creep and recovery curve of an ideally viscous material (according to NEWTON)
39 Viscoelastic liquids and solids The reaction of viscoelastic liquids on applied shear stress shows characteristics of both elastic and viscous strain. A partial recovery by the elastic portion γ E can be observed, but the portion of viscous strain γ V remains. γ γ E γ V t 0 t 2 t 4 t [s] γ E Elastic portion (recovery) γ V Viscous portion Fig. 720: Creep and recovery curve of a viscoelastic liquid In a viscoelastic solid, a delayed but complete recovery can be observed, i.e. γ V is almost zero. A material shall now be scrutinised which consists of macromolecules (parallel connection of spring 2 and damper 2) linked by springs (spring 1) in a highly viscous oil (damper 3). This model is also known as the BURGER model. Fig. 721: BURGER model
40 39 The applied shear stress initially leads to a spontaneous jump in strain (dilatation of spring elements 1 which are situated in the orientation of the strain), the strain rate then drops. During that time the macromolecules are oriented, the twisted springs tensioned and the macromolecules stretched up to their mechanically maximal possible size (delayed viscoelastic strain of spring 2 and damper 2). If more force is applied, the strain will again increase linearly if the macromolecules are irreversible disentangled and caused to flow with the viscous matrix mass (viscous strain of damper 3). If the test duration is long enough, all dampers and springs finally show maximum dilatation. During the relieve phase, two types of recovery take place. Spring 1 returns to its original tension immediately (elastic recovery), and the parallel connection of spring 2 and damper 2 recovers with a delay (viscoelastic recovery). Damper 3 remains fully displaced, so that a partial strain is maintained. If this remaining strain is very small (γ V near 0 %), the material is called a viscoelastic solid, otherwise it is a viscoelastic liquid. Creep curve (t 0 to t 2 ) Recovery curve (t 2 to t 4 ) γ 1... Purely elastic strain (spring 1) γ 2... Viscoelastic strain (parallel connection of spring 2 and damper 2) γ 3... Purely viscous strain (damper 3) γ max Maximum strain: γ 1 + γ 2 + γ 3 β.. Gradient angle of the strain curve on achievement of the stationary flow condition (depending on the viscosity of the strained material) γ E Elastic recovery portion Viscous recovery portion γ V Fig. 722: Creep and recovery curve with analysed parameters
41 40 In the load phase, unstationary flowing occurs in the linearly viscoelastic range between the points of time, t 0 and t 1. The viscosity here depends on the applied shear stress and time. ( τ,t) η = f x Stationary viscous flowing is observed between the points of time, t 1 and t 2. The viscosity does no longer depend on the elapsed loading time. ( ) η = f τ x The zero viscosity η 0 corresponds with the behaviour of damper 3 in the BURGER model (see Fig. 713). It can be determined as η 0 = τ γ x 3 = τ x tan β where the shear rate γ 3 = dγ / dt = tan β If determined at smallest shear rates, the zero viscosity η 0 is a material constant, which contains information e.g. about the molecular weight of nonnetworked macromolecules. In creep tests a constant shear stress is applied and the timedependent strain is measured. Mathematically, the relation between stress and strain can be expressed as follows: γ( t) = J(t) τ x This equation introduces the timedependent compliance factor J(t). Like the zero viscosity, it is a materialspecific quantity. It is a measure of the softness or flexibility of a material. The greater the compliance the more can the material be strained under the application of a certain shear stress. J(t) = γ(t) / t x in [Pa]
42 41 8 Measuring geometries in a rotation viscometer The measuring systems used in a rotation viscometer usually consist of a rotating and a rigid part. The rotating plunger is turned at either a preset speed or a preset torque. Two measuring principles are distinguished in coaxial measuring systems: (1) The SEARLE principle Rotating plunger and resting cup (or bottom plate) (2) The COUETTE principle Rotating cylinder (or bottom plate) and resting plunger Measuring systems which employ the COUETTE principle have drawbacks when it comes to temperature control, because it is more difficult technically to seal a rotating face than a fixed one. This is why the use of COUETTE systems is often restricted to low speeds. Fig. 81: Cylinder measuring arrangement Cylinder measuring arrangement according to the SEARLE principle according to the COUETTE principle
43 Coaxial cylinder measuring systems DIN describes the coaxial measuring system. Coaxial means that rotating member and resting member of the measuring system are disposed on one rotation axis. Such cylinder measuring systems are also known as concentric measuring systems. The terms of the parallel plate model can be applied to the round cylinder, if its surface area is idealised as many small plane faces. v(r) R i R a R i... Radius of the plunger (inner cylinder) R a... Radius of the cup (outer cylinder) r... Distance of a layer of the liquid from the rotation axis v(r)... Distribution of the circumferential speed in the measuring gap Fig. 82: Crosssection through a Searle cylinder measuring system The shear stress distribution τ(r) and the shear rate distribution (r) are dependent on the radii of the measuring system. In order to obtain nearlinear distributions (r) and τ(r), the measuring gap must not be too large. DIN thus specifies a maximum ratio of radii δ = R a /R i In other words, the DIN standard defines the ratio of radii, but not the absolute radii or gap size. The ratio of radii δ = R a /R i is specified in the DIN standard to be 1.1, preferably
44 43 Coaxial cylinder measuring system according to DIN α L.. Length of the plunger (inner cylinder) L.. Immersed skirt length L.. Distance between bottom edge of plunger and cup base R i... Radius of the plunger (inner cylinder) R a.. Radius of the cup (outer cylinder) R s... Radius of the plunger skirt α... Opening angle of the plunger cone Fig. 83: Cylinder measuring system according to DIN / ISO 3219 DIN prescribes the following geometrical arrangement for cylinder measuring systems: Ratio of radii δ = R a /R i 1.1 (preferably ) 90 α 150 (preferably 120 ± 1 ) L / R i 3 (preferably 3.00) L 1 / R i 1 (preferably 1.00) L 2 / R i 1 (preferably 1.00) R s / R i 0.3 Calculation of the shear stress τ from the torque M (measuring systems according to DIN 53019) τ = M 3 R i M in [mnm], R i in [m], τ in [Pa] Calculation of the shear rate from the rotational speed n (measuring systems according to DIN 53019) = n n in [min 1 ], in [s 1 ]
45 Dualslit measuring systems according to DIN This special coaxial cylinder measuring system with a particularly large shear area was standardised to be able to investigate materials which have a very small viscosity (such as waterbased lacquers, for example). The plunger has the shape of a tube and the cup has a cylindrical core section. This dualslit measuring system thus takes advantage of two shear faces, an inner and an outer plunger surface. R 4 R 3 R 2 L R 1 Fig. 84: Dualslit measuring system according to DIN According to DIN 54453, ratio of radii: δ = R 4 / R 3 = R 2 / R immersed length: L 3 R 3
46 Coneplate measuring systems according to ISO 3219 In the coneplate measuring system, the material to be investigated is disposed between the bottom plate and the measuring cone. According to DIN 53018, the cone angle must be rather small in order to allow the simplified expression tan β = β (β in rad) to be applied. The cone angle of that measuring system is chosen such that for each point on the cone surface the ratio of angular speed and distance to the plate is constant. This means that there is a constant shear rate across the entire radius of the measuring cone. The tip of the cone must just touch the bottom plate in this geometry. In order to prevent the cone tip from wear and at the same time to provide the possibility to measure materials which contain fillers, most rheometer manufacturers lift the cone tip by a certain amount ( µm). Measuring cones with an angle of 1 are most widespread. However, in order to be more flexible when it comes to measuring materials which contain fillers, dispersions are often measured using cones with an angle of 4. This guarantees a laminar flow to be generated in the measuring gap despite the dispersed particles. As a rule of thumb, a laminar flow can be assumed as long as the particle diameter is five times smaller than the gap. In addition to a constant shear rate across the entire measuring gap, the coneplate measuring system has further advantages, such as high shear rates, small sample quantities and easy cleaning. In order to obtain accurate results of the measurements, it is of major importance to conduct them very carefully. The measuring cone must be adjusted such that its imaginary tip just touches the bottom measuring plate. Another point is that of filling the measuring system. It is filled correctly if the material under investigation is visible approx. 1 mm around the entire circumference of the cone. The material must not escape from the measuring gap or rest on top of the measuring cone during the measurement. flattened cone tip correct filling approx. 1 mm Fig. 85: Filling the coneplate measuring system and detail of a cutoff cone tip
47 46 R ß R... ß... Outer radius of the cone Opening angle of the cone Fig. 86: Coneplate measuring system according to ISO 3219 / DIN The area A in the parallel plate model corresponds with the cone area A = π R². The moving force is expressed as F = M / R Calculation of the shear stress τ from the torque M τ = 3 M 2π R 3 = G K M Torque M in [mnm], R i in [m], τ in [Pa] G K is a constant of the measuring system which depends on the cone radius. The larger the cone radius the greater is the sensitivity of the measuring system. Calculation of the shear rate The velocity v in the parallel plate model corresponds with the circumferential speed v = ω R in the rotating system. ω = 2π n / 60 where ω is the angular speed in [rad/s] und n the rotational speed in [min 1 ] Using the simplified expression tan β = β for small cone angles, the shear rate can be calculated from the rotational speed n according to the following equation: = ω β = k n where k is a conversion factor which is independent of the cone angle. At a cone angle of 1 k = 6, at an angle of 2 k = 3 and at an angle of 4 k = This means that at a constant rotational speed the shear rate is the higher the smaller the cone angle. Angles are given in [rad] or [degree], where 2π rad = 360 i.e. 1 rad = 57.3 and 1 = rad.
48 Plateplate measuring systems The plateplate measuring system consists of two parallel plates. It is characterised by the plate radius R and the variable distance h between the plates. The material under investigation is disposed between the two plates. DIN specifies that the plate distance h shall be much smaller than the radius of the measuring plate. A gap of between 0.3 mm and 3 mm is recommended. Plateplate measuring devices are used if the material under investigation contains large filler particles. The gap should be determined such that it is at least five times as large as the largest particles contained in the material. The shear rate is not constant across the entire plate radius, like in the coneplate system, but there is a relatively large shear rate range. The shear rate in the centre of the upper measuring plate is zero. The specified shear rate is always that related to the outer radius R of the measuring plate, that is the maximum shear gradient. R h R... H... Radius of the measuring plate Distance (gap) between the upper and lower measuring plate Fig. 87: Plateplate measuring system The area A in the parallel plate model corresponds with the rotating area A of the upper measuring plate, where A = π R 2. The moving force is expressed as F = M / R. Calculation of the shear stress τ from the torque M τ 3 M ( R) = = G M 2π R 3 P Torque M in [mnm], R in [m], τ in [Pa] G P is a constant of the measuring system which depends on the plate radius and the distance h. The larger the plate radius the greater is the sensitivity of the measuring system.
49 48 Calculation of the shear rate The plate distance h in the parallel plate model corresponds with the distance h between the upper and lower measuring plate; the velocity v in the parallel plate model corresponds with the circumferential speed v = ω R in the rotating system. ω = 2π n / 60 where ω is the angular speed in [rad/s] und n the rotational speed in [min 1 ] In contrast to the coneplate measuring system, the shear rate depends on the radius. It is zero in the centre of the plate (r = 0), has a maximum at the edge of the plate (r = R) and shows a linear gradient. ( R) = v h = ω R h At a constant angular speed ω or rotational speed n, if the plate distance h is increased the shear rate in the measuring gap will fall.
How to measure the shear viscosity properly?
testxpo Fachmesse für Prüftechnik 10.13.10.2016 How to measure the shear viscosity properly? M p v Rotation Capillary Torsten Remmler, Malvern Instruments Outline How is the Shear Viscosity defined? Principle
More informationDynamic (absolute) Viscosity
Viscosity Taken from: http://www.engineeringtoolbox.com/dynamicabsolutekinematicviscosityd_412.html The viscosity of a fluid is an important property in the analysis of liquid behavior and fluid motion
More informationCustom Search Sponsored Links
Dynamic, Absolute and Kinematic Viscosity An introduction to dynamic, absolute and kinematic viscosity and how to convert between CentiStokes (cst), CentiPoises (cp), Saybolt Universal Seconds (SSU), degree
More informationCharacterization of the structure at rest in foods (Example: Ketchup)
Characteriszation of the structure at rest / page 1 Characterization of the structure at rest in foods (Example: Ketchup) by Thomas Mezger, Physica Messtechnik GmbH, Ostfildern (Stuttgart), Germany Overview
More informationArticle for the 29 th Sensing Forum
Article for the 29 th Sensing Forum Characteristics of Tuningfork Vibration Rheometer RHEOVISCO RV10000 Presented by: Naoto Izumo, Yuji Fukami, and Masahiro Kanno R&D Division 5, A&D Company, Limited
More informationFluid Mechanics II Viscosity and shear stresses
Fluid Mechanics II Viscosity and shear stresses Shear stresses in a Newtonian fluid A fluid at rest can not resist shearing forces. Under the action of such forces it deforms continuously, however small
More informationA BASIC INTRODUCTION TO RHEOLOGY
A BASIC INTRODUCTION TO RHEOLOGY All rights reserved. No part of this manual may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying, recording or
More information1912 MEASUREMENT OF HARDNESS OF SEMISOLIDS
BRIEFING 1912 Measurement of Hardness of Semisolids. This proposed new chapter summarizes the mathematical models used to quantify the viscoelastic properties of semisolids, as well as the most common
More information1. Introduction, fluid properties (1.1, 2.8, 4.1, and handouts)
1. Introduction, fluid properties (1.1, 2.8, 4.1, and handouts) Introduction, general information Course overview Fluids as a continuum Density Compressibility Viscosity Exercises: A1 Fluid mechanics Fluid
More informationViscoelasticity. Basic Notions & Examples. Formalism for Linear Viscoelasticity. Simple Models & Mechanical Analogies. Nonlinear behavior
Viscoelasticity Basic Notions & Examples Formalism for Linear Viscoelasticity Simple Models & Mechanical Analogies Nonlinear behavior Viscoelastic Behavior Generic Viscoelasticity: exhibition of both
More informationNon Newtonian Fluid Dynamics
PDHonline Course M417 (3 PDH) Non Newtonian Fluid Dynamics Instructor: Paul G. Conley, PE 2012 PDH Online PDH Center 5272 Meadow Estates Drive Fairfax, VA 220306658 Phone & Fax: 7039880088 www.pdhonline.org
More informationUniversity Graz / Austria Institut für Chemie Volker Ribitsch
University Graz / Austria Institut für Chemie Volker Ribitsch 1 Rheology Oscillatory experiments Dynamic experiments Deformation of materials under nonsteady conditions in the linear viscoelastic range
More informationNONNEWTONIAN FLUIDS. What are they? AND POLYMERS
NONNEWTONIAN FLUIDS What are they? AND POLYMERS VOCABULARY NonNewtonian Dilatant rigid Thixotropic does NOT follow the laws of physics as described by Newton adding energy (shear force) makes a liquid
More informationInterfacial Shear Rheology of Films Formed by Coffee
ANNUAL TRANSACTIONS OF THE NORDIC RHEOLOGY SOCIETY, VOL. 16, 2008 Interfacial Shear Rheology of Films Formed by Coffee Patrick Heyer, Jörg Läuger Anton Paar Germany GmbH, HelmuthHirthStrasse 6, 73760
More informationWell prepared  good results
APPLICATION NOTE Well prepared  good results No. V248 Authors Cornelia KüchenmeisterLehrheuer and Klaus Olddörp Thermo Fisher Scientific, Karlsruhe, Germany Introduction In recent years the demands
More informationFluid Flow. Fundamentals of Rheology. Rheology is the science of deformation and flow. Food rheology is the material science of food
Fluid Flow Outline Fundamentals and applications of rheology Shear stress and shear rate Viscosity and types of viscometers Rheological classification of fluids Apparent viscosity Effect of temperature
More informationRHEOLOGY Principles, Measurements, and Applications. Christopher W. Macosko
RHEOLOGY Principles, Measurements, and Applications I 560815'79~5 1994 VCH Publishers. Inc. New York Part I. CONSTITUTIVE RELATIONS 1 1 l Elastic Solid 5 1.1 Introduction 5 1.2 The Stress Tensor 8 1.2.1
More informationCENG 501 Examination Problem: Estimation of Viscosity with a Falling  Cylinder Viscometer
CENG 501 Examination Problem: Estimation of Viscosity with a Falling  Cylinder Viscometer You are assigned to design a fallingcylinder viscometer to measure the viscosity of Newtonian liquids. A schematic
More informationRheological Measurements of Cementitious Suspensions Using a Grooved Measuring Device
ANNUAL TRANSACTIONS OF THE NORDIC RHEOLOGY SOCIETY, VOL. 17, 2009 Rheological Measurements of Cementitious Suspensions Using a Grooved Measuring Device Helge Hodne 1, Arild Saasen 1,2, and Jone Haugland
More informationChapter 3 NonNewtonian fluid
Chapter 3 NonNewtonian fluid 31. Introduction: The study of the deformation of flowing fluids is called rheology; the rheological behavior of various fluids is sketchen Figure 31. Newtonian fluids,
More informationRheology step 1. Principles of Rheology and its Measurement techniques. Panta Rei. TRAINING. Viscosity, Elasticity and Viscoelasticity
Rheology step 1 Principles of Rheology and its Measurement techniques Viscosity, Elasticity and Viscoelasticity Fresh After 12 h Panta Rei. +46 709787805 www.reokonsa.com 1 (8) For whom: Rheology is the
More informationThe Large Amplitude Oscillatory Strain Response of Aqueous Foam: Strain Localization and Full Stress Fourier Spectrum
The Large Amplitude Oscillatory Strain Response of Aqueous Foam: Strain Localization and Full Stress Fourier Spectrum By F. Rouyer, S. CohenAddad, R. Höhler, P. Sollich, and S.M. Fielding The European
More informationRHEOLASER LAB MICRORHEOLOGY & END USE PROPERTIES ANALYSIS. MICRORHEOLOGY
RHEOLASER LAB & END USE PROPERTIES ANALYSIS A NEW RHEOLOGY APPROACH TO CHARACTERISE ENDUSE PROPERTIES THE FIRST READY TO USE & ENDUSE PROPERTIES ANALYSER Rheolaser Rheolaser is the first Lab readytouse
More informationRHEOLOGY AND RHEOLOGICAL MEASUREMENTS
RHEOLOGY AND RHEOLOGICAL MEASUREMENTS 1. Introduction Rheology is the science of the deformation and flow of matter. It is concerned with the response of materials to applied stress. That response may
More informationFundamentals of Rheology Science of Deformation and Flow Homer Jamasbi, Ph.D. Elementis Specialties
Fundamentals of Rheology Science of Deformation and Flow Homer Jamasbi, Ph.D. Elementis Specialties Introduction Rheology is the study of how materials deform and flow under the influence of external forces.
More informationLecture 2. Simple shear devices. Simple shear devices 2. Simple shear devices 3. Moving plate. Velocity V. Force F. Area A. height h.
Lecture 2 Rheometry Simple shear devices Steady shear viscosity Normal stresses Oscillating shear Extensional viscosity Scalings Nondimensional parameter Simple shear devices Conceptual device for simple
More informationDynamic Mechanical Analysis of Solid Polymers and Polymer Melts
Polymer Physics 2015 Matilda Larsson Dynamic Mechanical Analysis of Solid Polymers and Polymer Melts Polymer & Materials Chemistry Introduction Two common instruments for dynamic mechanical thermal analysis
More informationMeasuring structure of low viscosity fluids in oscillation using rheometers with and without a separate torque transducer
ANNUAL RANSACONS OF HE NORDC RHEOLOGY SOCEY, VOL., 003 Measuring structure of low viscosity fluids in oscillation using rheometers with and without a separate torque transducer Aly Franck A nstruments,
More informationRheology of strongly sedimenting magnetite suspensions
ANNUAL TRANSACTIONS OF THE NORDIC RHEOLOGY SOCIETY, VOL. 13, 05 Rheology of strongly sedimenting magnetite suspensions Jan Gustafsson1, Martti Toivakka1, and Kari K. Koskinen2 1 Laboratory of Paper Coating
More informationRheological Properties of Fresh Building Materials
Application Note V217 Rheological Properties of Fresh Building Materials Dipl.Ing. Michael Haist Univ.Prof. Dr.Ing. Harald S. Müller, Institute of Concrete Structures and Building Materials, University
More informationSTUDY OF RHEOLOGICAL PROPERTIES OF BITUMINOUS BINDERS IN MIDDLE AND HIGH TEMPERATURES
Vol. 12, Issue 1/2016, 1320 DOI: 10.1515/cee20160002 STUDY OF RHEOLOGICAL PROPERTIES OF BITUMINOUS BINDERS IN MIDDLE AND HIGH TEMPERATURES Eva REMIŠOVÁ 1,*, Viera ZATKALIKOVÁ 2, František SCHLOSSER
More informationObjective Methods of Food Analysis. Brookfield Viscometer. Brookfield viscometer
Objective Methods of Food Analysis Brookfield Viscometer Measures the thickness, or viscosity, of liquid dispersions such as salad dressings. A measure of liquid texture. Brookfield viscometer 1 Compensating
More informationApplied Rheology Richard R. Eley, Ph.D. Senior Scientist ICI Paints Sprague Road Strongsville, OH 44136
Applied Rheology Richard R. Eley, Ph.D. Senior Scientist ICI Paints 16651 Sprague Road Strongsville, OH 44136 The science of Rheology by definition is the study of the deformation and flow behavior of
More information1 Rheology of Disperse Systems
7 1 Rheology of Disperse Systems Norbert Willenbacher and Kristina Georgieva 1.1 Introduction The rheology of disperse systems is an important processing parameter. Being able to characterize and manipulate
More informationInterfacial dynamics
Interfacial dynamics Interfacial dynamics = dynamic processes at fluid interfaces upon their deformation Interfacial rheological properties: elasticity, viscosity, yield stress, Relation between macroscopic
More informationIndepth analysis of viscoelastic properties thanks to Microrheology: noncontact rheology
Indepth analysis of viscoelastic properties thanks to Microrheology: noncontact rheology Application All domains dealing with soft materials (emulsions, suspensions, gels, foams, polymers, etc ) Objective
More informationSECOND ENGINEER REG. III/2 APPLIED MECHANICS
SECOND ENGINEER REG. III/2 APPLIED MECHANICS LIST OF TOPICS Static s Friction Kinematics Dynamics Machines Strength of Materials Hydrostatics Hydrodynamics A STATICS 1 Solves problems involving forces
More informationLes Houches School of Foam: Rheology of Complex Fluids
Les Houches School of Foam: Rheology of Complex Fluids Andrew Belmonte The W. G. Pritchard Laboratories Department of Mathematics, Penn State University 1 Fluid Dynamics (tossing a coin) Les Houches Winter
More informationHomework of chapter (1) (Solution)
بسم اهلل الرمحن الرحيم The Islamic University of Gaza, Civil Engineering Department, Fluid mechanicsdiscussion, Instructor: Dr. Khalil M. Al Astal T.A: Eng. Mohammed H El Nazli Eng. Sarah R Rostom First
More informationOPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION
OPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION Luca Barbaresi, Federica Morandi, Juri Belcari, Andrea Zucchelli and Alice Speranza University
More informationSoft matters end use properties analysis thanks to Microrheology
Soft matters end use properties analysis thanks to Microrheology Formulaction, 10 impasse Borde Basse, 31240 L Union, France, www.formulaction.com Abstract. We present a new technique of passive microrheology
More informationMODIFICATION OF THE CONCRETE RHEOMETER TO DETERMINE RHEOLOGICAL PARAMETERS OF SELF CONSOLIDATING CONCRETE VANE DEVICE
MODIFICATION OF THE CONCETE HEOMETE TO DETEMINE HEOLOGICAL PAAMETES OF SELF CONSOLIDATING CONCETE VANE DEVICE Ammar Yahia and Kamal H. Khayat Department of Civil Engineering, Université de Sherbrooke,
More informationCHARACTERIZATION OF RHEOLOGICAL PROPERTIES OF SEMISOLID MATERIALS USED AS THERMAL INTERFACES. PART I: A BRIEF REVIEW
Journal of Engineering Studies and Research Volume 21 (2015) No. 4 14 CHARACTERIZATION OF RHEOLOGICAL PROPERTIES OF SEMISOLID MATERIALS USED AS THERMAL INTERFACES. PART I: A BRIEF REVIEW FLORINACARMEN
More informationBME 419/519 Hernandez 2002
Vascular Biology 2  Hemodynamics A. Flow relationships : some basic definitions Q v = A v = velocity, Q = flow rate A = cross sectional area Ohm s Law for fluids: Flow is driven by a pressure gradient
More informationContents. Microfluidics  Jens Ducrée Physics: Laminar and Turbulent Flow 1
Contents 1. Introduction 2. Fluids 3. Physics of Microfluidic Systems 4. Microfabrication Technologies 5. Flow Control 6. Micropumps 7. Sensors 8. InkJet Technology 9. Liquid Handling 10.Microarrays 11.Microreactors
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationFRANK OHENE Department of Chemistry Grambliig State University Grambling, LA 71245
i f i i EFFECT OF COAL BENEFICIATION PROCESS ON RHEOLOGY/ATOMIZATIONOF COAL WATER SLURRIES. Quarterly Progress Report Aprill, 1996 June 30, 1996 FRANK OHENE Department of Chemistry Grambliig State University
More informationUSE OF RHEOLOGY AS A DEVELOPING AND TROUBLESHOOTING TOOL FOR PSA APPLICATIONS.
USE OF RHEOLOGY AS A DEVELOPING AND TROUBLESHOOTING TOOL FOR PSA APPLICATIONS. Michael DeFrancisis, Applications Engineer, Henkel, Bridgewater, NJ Yayun Liu, Senior Development Scientist, Henkel, Bridgewater,
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationThe Physics of NonNewtonian Fluids
The Physics of NonNewtonian Fluids M. Grogan 10. April 2006 [1][4] R. Fox, A. McDonald, P. Pritchard, Introduction to Fluid Mechanics, 6 th Ed. 2004 Wiley, United States of America. p3, p27. [2],[3] B
More informationUniversal Viscosity Curve Theory
TM Universal Viscosity Curve Theory Turbine Flow Meters and Flow Viscosity Introduction Like any transducer, a turbine flow meter is sensitive to physical parameters other than the one which is of interest.
More informationChapter 13 ELASTIC PROPERTIES OF MATERIALS
Physics Including Human Applications 280 Chapter 13 ELASTIC PROPERTIES OF MATERIALS GOALS When you have mastered the contents of this chapter, you will be able to achieve the following goals: Definitions
More informationNonlinear Viscoelastic Behaviors of Different Types of O/W EmulsionBased Mayonnaises in Several Shear Flow Fields
ANNUAL TRANSACTIONS OF THE NORDIC RHEOLOGY SOCIETY, VOL 19, 211 Nonlinear Viscoelastic Behaviors of Different Types of O/W EmulsionBased Mayonnaises in Several Shear Flow Fields HyeJin Ahn and KiWon
More informationHoney Coiling  A Study on the Gravitational Regime of Liquid Rope Coiling
Honey Coiling  A Study on the Gravitational Regime of Liquid Rope Coiling Patrick Meister, MNG Rämibühl, patrickmeister@ymail.com 1 Introduction We report on the coiling motion a falling stream of viscous
More informationModeling Mechanical Systems
Modeling Mechanical Systems Mechanical systems can be either translational or rotational. Although the fundamental relationships for both types are derived from Newton s law, they are different enough
More informationTorsion Stresses in Tubes and Rods
Torsion Stresses in Tubes and Rods This initial analysis is valid only for a restricted range of problem for which the assumptions are: Rod is initially straight. Rod twists without bending. Material is
More informationSpreading of a HerschelBulkley Fluid Using Lubrication Approximation
Journal of Undergraduate Research 7, 114 (214) Spreading of a HerschelBulkley Fluid Using Lubrication Approximation Nadiya Klep 1Department of Material Science and Engineering Clemson University, Clemson,
More informationCalculation of Power and Flow Capacity of Rotor / Stator Devices in VisiMix RSD Program.
Calculation of Power and Flow Capacity of Rotor / Stator Devices in VisiMix RSD Program. L.N.Braginsky, D.Sc. (Was invited to be presented on the CHISA 201013th Conference on Process Integration, Modelling
More informationTHE INFLUENCE OF TIME OF RHEOLOGICAL PARAMETERS OF FRESH CEMENT SLURRIES**
http://dx.doi.org/10.7494/drill.2014.31.1.123 **, Andrzej Gonet*, * THE INFLUENCE OF TIME OF RHEOLOGICAL PARAMETERS OF FRESH CEMENT SLURRIES** 1. INTRODUCTION The rheological properties of sealing slurries
More informationMeasurement and Prediction of Fluid Viscosities at High Shear Rates
Chapter 5 Measurement and Prediction of Fluid Viscosities at High Shear Rates Jeshwanth K. Rameshwaram and Tien T. Dao Additional information is available at the end of the chapter http://dx.doi.org/10.5772/54282
More informationPractical 1P9 Polymers  Molecular weight effects
Practical 1P9 Polymers  Molecular weight effects What you should learn from this practical Science The main theme of the Polymer Synthesis lectures is that molecular weight, and the ability to control
More informationFORMULA SHEET. General formulas:
FORMULA SHEET You may use this formula sheet during the Advanced Transport Phenomena course and it should contain all formulas you need during this course. Note that the weeks are numbered from 1.1 to
More information19 Rheology Chapter Objectives At the conclusion of this chapter the student should be able to:
19 Rheology Chapter Objectives At the conclusion of this chapter the student should be able to: 1. Define rheology, provide examples of fluid pharmaceutical products exhibiting various rheologic behaviors,
More information150A Review Session 2/13/2014 Fluid Statics. Pressure acts in all directions, normal to the surrounding surfaces
Fluid Statics Pressure acts in all directions, normal to the surrounding surfaces or Whenever a pressure difference is the driving force, use gauge pressure o Bernoulli equation o Momentum balance with
More informationEXAMPLE SHEET FOR TOPIC 3 AUTUMN 2013
EXAMPLE SHEET FOR TOPIC ATMN 01 Q1. se dimensional analysis to investigate how the capillary rise h of a liquid in a tube varies with tube diameter d, gravity g, fluid density ρ, surface tension σ and
More informationResistance Coefficients for NonNewtonian Flows in Pipe Fittings
Resistance Coefficients for NonNewtonian Flows in Pipe Fittings Veruscha Fester 1, Paul Slatter 2 and Neil Alderman 3 7 1 Cape Peninsula University of Technology, 2 Royal Melbourne Institute of Technology,
More informationEntanglements. M < M e. M > M e. Rouse. Zeroshear viscosity vs. M (note change of slope) Edwards degennes Doi. Berry + Fox, slope 3.4.
Entanglements Zeroshear viscosity vs. M (note change of slope) M < M e Rouse slope 3.4 M > M e Edwards degennes Doi slope 1 Berry + Fox, 1968 Question: Which factors affect the Me: T, P, M, flexibility,
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More informationClass XI Physics. Ch. 9: Mechanical Properties of solids. NCERT Solutions
Downloaded from Class XI Physics Ch. 9: Mechanical Properties of solids NCERT Solutions Page 242 Question 9.1: A steel wire of length 4.7 m and crosssectional area 3.0 10 5 m 2 stretches by the same amount
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationUsing Rheological Properties to Evaluate Storage Stability and Setting Behaviors of Emulsified asphalts
Using Rheological Properties to Evaluate Storage Stability and Setting Behaviors of Emulsified asphalts Huachun Zhai, Delmar Salomon * and Eric Milliron Idaho Asphalt Supply, Inc. 2627 Brandt Ave., Nampa,
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationParticle removal in linear shear flow: model prediction and experimental validation
Particle removal in linear shear flow: model prediction and experimental validation M.L. Zoeteweij, J.C.J. van der Donck and R. Versluis TNO Science and Industry, P.O. Box 155, 600 AD Delft, The Netherlands
More informationOscillatory Motion SHM
Chapter 15 Oscillatory Motion SHM Dr. Armen Kocharian Periodic Motion Periodic motion is motion of an object that regularly repeats The object returns to a given position after a fixed time interval A
More informationComparison between the viscoelastic dampers And Magnetorheological dampers and study the Effect of temperature on the damping properties
Comparison between the viscoelastic dampers And Magnetorheological dampers and study the Effect of temperature on the damping properties A.Q. Bhatti National University of Sciences and Technology (NUST),
More informationContents. Dynamics and control of mechanical systems. Focus on
Dynamics and control of mechanical systems Date Day 1 (01/08) Day 2 (03/08) Day 3 (05/08) Day 4 (07/08) Day 5 (09/08) Day 6 (11/08) Content Review of the basics of mechanics. Kinematics of rigid bodies
More informationPolymer Rheology. P Sunthar. Department of Chemical Engineering Indian Institute of Technology, Bombay Mumbai , India
Polymer Rheology P Sunthar Department of Chemical Engineering Indian Institute of Technology, Bombay Mumbai 400076, India P.Sunthar@iitb.ac.in 05 Jan 2010 Introduction Phenomenology Modelling Outline of
More informationTHE RHEOLOGICAL BEHAVIOR OF CONCENTRATED ORANGE JUICE
HEFAT2014 10 th International Conference on Heat Transfer, Fluid Mechanics and Thermodynamics 14 26 July 2014 Orlando, Florida THE RHEOLOGICAL BEHAVIOR OF CONCENTRATED ORANGE JUICE Kar F. and Kaya B. A.
More informationShell Balances in Fluid Mechanics
Shell Balances in Fluid Mechanics R. Shankar Subramanian Department of Chemical and Biomolecular Engineering Clarkson University When fluid flow occurs in a single direction everywhere in a system, shell
More informationTerraMechanical Simulation Using Distinct Element Method
Shinya Kanou Masaharu Amano Yuji Terasaka Norihisa Matsumoto Tatsuo Wada To our company that designs and manufactures equipment for handling soil and rock, analyzing the interaction or contact between
More informationRELIABILITY OF RHEOMETRIC MEASUREMENTS IN BITUMENS BY MEANS OF DYNAMIC SHEAR RHEOMETERS
RELIABILITY OF RHEOMETRIC MEASUREMENTS IN BITUMENS BY MEANS OF DYNAMIC SHEAR RHEOMETERS Antonio MONTEPARA, University of Parma, Parma, Italy Felice GIULIANI, University of Parma, Parma, Italy 1. INTRODUCTION
More informationGuide to Rheological Nomenclature: Measurements in Ceramic Particulate Systems
NIST Special Publication 946 Guide to Rheological Nomenclature: Measurements in Ceramic Particulate Systems Vincent A. Hackley and Chiara F. Ferraris G* = G + jg Tan δ = G G *G** ä G" G' ó amplitude ó
More informationFigure 3: Problem 7. (a) 0.9 m (b) 1.8 m (c) 2.7 m (d) 3.6 m
1. For the manometer shown in figure 1, if the absolute pressure at point A is 1.013 10 5 Pa, the absolute pressure at point B is (ρ water =10 3 kg/m 3, ρ Hg =13.56 10 3 kg/m 3, ρ oil = 800kg/m 3 ): (a)
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationMSE 383, Unit 33. Joshua U. Otaigbe Iowa State University Materials Science & Engineering Dept.
Dynamic Mechanical Behavior MSE 383, Unit 33 Joshua U. Otaigbe Iowa State University Materials Science & Engineering Dept. Scope Why DMA & TTS? DMA Dynamic Mechanical Behavior (DMA) Superposition Principles
More informationSome frequently used models for nonnewtonian fluids
Some frequently used models for nonnewtonian fluids malek@karlin.mff.cuni.cz Mathematical Institute Charles University 18 March 2011 Fluid Viscosity [cp] Air (at 18 C) 0.02638 Benzene 0.5 Water (at 18
More informationApplied physical pharmacy 10. Rheology
Applied physical pharmacy 10. Rheology Sungkyunkwan University, School of Pharmacy Physical Pharmacy Lab Gyoung Won Kim CONTENTS Introduction Newtonian system Non  Newtonian system Thixotropy Viscoelasticity
More informationMeasuring the rheology of thermoplastic polymer melts
Measuring the rheology of thermoplastic polymer melts Using rotational and capillary rheometry to characterize polymer melts RHEOLOGY AND VISCOSITY Introduction Rheology is the science of studying the
More informationContents XVII. Preface
V Preface XVII 1 General Introduction 1 1.1 Suspensions 1 1.2 Latexes 2 1.3 Emulsions 2 1.4 Suspoemulsions 3 1.5 Multiple Emulsions 3 1.6 Nanosuspensions 4 1.7 Nanoemulsions 4 1.8 Microemulsions 5 1.9
More informationME3250 Fluid Dynamics I
ME3250 Fluid Dynamics I Section I, Fall 2012 Instructor: Prof. Zhuyin Ren Department of Mechanical Engineering University of Connecticut Course Information Website: http://www.engr.uconn.edu/~rzr11001/me3250_f12/
More informationEmulsion Processing  Homogenization 
Emulsion Processing  Homogenization  Jochen Weiss *Food Structure and Functionality Laboratories Department of Food Science & Biotechnology University of Hohenheim Garbenstrasse 21, 70599 Stuttgart,
More informationRHEOLOGY OF GMELINA AND RUBBER SEEDS OIL LUBRICANTS
Journal of Novel Applied Sciences Available online at www.jnasci.org 2013 JNAS Journal20132S4/11431149 ISSN 23225149 2013 JNAS RHEOLOGY OF GMELINA AND RUBBER SEEDS OIL LUBRICANTS Oseni M I 1,Ette
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationFriction Factors and Drag Coefficients
Levicky 1 Friction Factors and Drag Coefficients Several equations that we have seen have included terms to represent dissipation of energy due to the viscous nature of fluid flow. For example, in the
More informationNovel method for online rheology measurement in manufacturing of non Newtonian liquids
Novel method for online rheology measurement in manufacturing of non Newtonian liquids Fridolin Okkels, Anders L. Østergård, Mohammad Amin Mohammadifar 2 Fluidan ApS, Kgs. Lyngby, Denmark 2 National
More informationEffect of Temperature and Pressure on Rheological Measurements of Cement Slurries
ANNUAL TRANSACTIONS OF THE NORDIC RHEOLOGY SOCIETY, VOL. 22, 2014 Effect of Temperature and Pressure on Rheological Measurements of Cement Slurries Kristján Friðrik Alexandersson 1 and Sunna Ólafsdóttir
More informationHIGH PRESSURE CAPILLARY RHEOMETRY ON WOOD PLASTIC COMPOSITES WITH VARIATION OF WOOD CONTENT AND MATRIX POLYMER ABSTRACT
URN (Paper): urn:nbn:de:gbv:ilm12014iwk170:9 58 th ILMENAU SCIENTIFIC COLLOQUIUM Technische Universität Ilmenau, 08 12 September 2014 URN: urn:nbn:de:gbv:ilm12014iwk:3 HIGH PRESSURE CAPILLARY RHEOMETRY
More informationTimeDependent Rheology of Concentrated Xanthan Gum Solutions
ANNUAL TRANSACTIONS OF THE NORDIC RHEOLOGY SOCIETY, VOL 19, 211 TimeDependent Rheology of Concentrated Xanthan Gum Solutions JiSeok Lee and KiWon Song* Department of Organic Material Science and Engineering,
More informationStress, Strain, and Viscosity. San Andreas Fault Palmdale
Stress, Strain, and Viscosity San Andreas Fault Palmdale Solids and Liquids Solid Behavior: Liquid Behavior:  elastic  fluid  rebound  no rebound  retain original shape  shape changes  small deformations
More informationQuiz 1. Introduction to Polymers
100406 Quiz 1. Introduction to Polymers 1) Polymers are different than lowmolecular weight oligomers. For example an oligomeric polyethylene is wax, oligomeric polystyrene is similar to naphthalene (moth
More information